Comparative Study of Lead (II) Removal from Aqueous Solution ... (OPS), as potential raw materials for the preparation .... standard test of ASTM D 3838-80 .
J. T. Nwabanne, P. K. Igbokwe / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 4, July-August 2012, pp.1830-1838
Comparative Study of Lead (II) Removal from Aqueous Solution Using Different Adsorbents J. T. Nwabanne and P. K. Igbokwe Department of Chemical Engineering, Nnamdi Azikiwe University, P.M.B. 5025, Awka, Nigeria.
ABSTRACT Adsorption of lead(II) from wastewater effluents using indigenous cellulose based waste biomass, such as nipa palm nut (NPN), palmyra palm nut (PPN), oil palm empty fruit bunch (EFB), oil palm fibre (OPF), and oil palm shell (OPS), as potential raw materials for the preparation of activated carbons was studied. Chemical activation method was used in preparing the activated carbon. The influence of various factors namely pH, adsorbent dosage, contact time, initial ion concentration and adsorbent particle size was studied to identify the adsorption capacity of the adsorbents. The amount of Pb2+ adsorbed increased with increase in adsorbent dosage, and contact time and decreased with increase in particle size and initial ion concentration. The optimum pH was obtained at pH6 for all the adsorbents. The result of adsorption studies showed that activated carbons produced from OPS and NPN are the most efficient adsorbents for the removal of Pb2+ from aqueous solutions. Adsorption data were modeled using Langmuir, Freundlich, Temkin and Dubinin-Radushkevich equations. Equilibrium data fitted well to the Freundlich, Langmuir and Tempkin models. The equilibrium data were best described by Freundlich model. It is seen from the study that all the adsorbents can be used as low-cost adsorbents for the removal of Pb2+ from aqueous solution. Key words: Adsorption, lead, adsorbents, isotherm, removal, activated carbon
1. INTRODUCTION Activated carbons are the most widely used industrial adsorbent for removing pollutants from gaseous, aqueous and non aqueous streams, due to their uniquely powerful adsorption properties and the ability to readily modify their surface chemistry . Activated carbons are amorphous solid adsorbents that can be produced from almost all carbon-rich materials, including wood, fruit stones, peat, lignite, anthracite, shells and other raw materials . Its unique adsorption properties result from its high-surface area, adequate pore size distribution, broad range of surface functional groups, and relatively high mechanical strength. These unique characteristics are responsible for its
adsorptive properties, which are exploited in many different liquid-and gas-phase applications . There are two main methods for the preparation of activated carbons. These are physical and chemical activation methods. Physical activation occurs in two stages – thermal decomposition or carbonisation of the precursor and controlled gasification or activation of the crude char. The carbonisation process causes some increase in porosity, although this is generally insufficient for practical use, and serves to modify the pore structure inherent to the precursor, as opposed to creating it . During carbonization, most of the non-carbon elements such as oxygen, hydrogen, nitrogen and sulphur are eliminated as volatile gaseous products by the pyrolytic decomposition of the source raw material to produce a carbon skeleton possessing a latent pore structure [2, 4]. The activation process helps to develop further this structure by selective gasification of carbon, usually in temperature range of 600-12000C in steam, CO2 or O2 or mixtures of these. Chemical activation involves the treatment of the initial material with a dehydrating agent, such as sulphuric acid, phosphoric acid, zinc chloride, potassium hydroxide, or other substances, at temperatures varying from 400 to 10000C, followed by the elimination of the dehydrating agent by meticulous washing . With chemical activation, relevant reactions involve attack on the cellulosic structures in the precursor. Recently, preparation of activated carbons from agricultural by products has been given serious attention due to the growing interest in low cost activated carbons from renewable biomass, especially for applications concerning treatment of drinking water and wastewater . These agricultural wastes (waste biomass) impact negatively on the environment because of indiscriminate disposal of such wastes. Hence producing activated carbon from these wastes is an alternative method of waste reduction and reuse. The contamination of water by toxic metals through the discharge of industrial wastewater is becoming a serious environment problem in Nigeria. Heavy metals ions are reported as priority pollutants, due to their mobility in natural water ecosystems and due to their toxicity. The presence of these heavy metals in streams and surface waters has been responsible for several health problems with animals, plants and human beings. Lead is a
1830 | P a g e
J. T. Nwabanne, P. K. Igbokwe / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 4, July-August 2012, pp.1830-1838 pollutant that is present in drinking water and in air. In air, it is derived from lead emissions from automobiles because it is used as an anti knocking agent in the form of lead tetraethyl in gasoline. In water, lead is released in effluent from lead treatment and recovery industries, especially from lead battery manufacturing units. Lead is toxic to living organisms and if released into the environment can both accumulate and enter the food chain. Lead is known to cause mental retardations, reduces haemoglobin production necessary for oxygen transport and it interferes with normal cellular metabolism . Lead has damaging effects on body nervous system. Several methods such as ion exchange, solvent extraction, reverse osmosis, precipitation, and adsorption have been proposed for the treatment of wastewater contaminated with heavy metals . Among several chemical and physical methods, the adsorption onto activated carbon has been found to be superior to other techniques in water-re-use methodology because of its capability for adsorbing a broad range of different types of adsorbates efficiently, and its simplicity of design . The aim of this study is to compare the performance of these five adsorbents in the adsorption of lead (II) from aqueous solution.
2. MATERIALS AND METHODS 2.1 Sourcing and pre-treatment of raw materials The raw materials used for the preparation of activated carbon are oil palm shell (OPS), oil palm fibre (OPF), oil palm empty fruit bunch (EFB), nipa palm nut (NPN) and palmyra palm nut (PPN). Oil palm shell, oil palm fibre and oil palm empty fruit bunch were obtained from Ichida women co-operative oil processing mill, Ichida, Anambra State, Nigeria. Nipa palm nuts were obtained from a mangrove in Nkpogu village, Rivers State while Palmyra palm nuts were obtained from Nnamdi Azikiwe University, Awka, Anambra State, Nigeria. The raw materials were washed several times using de-ionized water to remove all traces of impurities, oil, dirt, dust, etc. The materials were dried in the sun for 72 hours to remove excess water until constant weight was obtained. 2.2 Production of activated carbon The washed and dried raw materials were ground into fine particles using a Jencod grinding machine and sieved to a particle size of 300µm. 200g of sample was impregnated with concentrated orthophosphoric acid at the acid/precursor ratio of 0.4:1 (wt basis) for OPS and 2:1 for other materials. The impregnated samples were dried in an oven at 1200C for 24hrs. The dried samples were carbonized in a Muffle furnace for 1hr at 5000C for NPN, 2hrs at 5000C for PPN and 2hrs at 8000C for EFB, OPF and OPS. After cooling to the ambient temperature, the samples were washed with de-ionized water several times until pH 6-7, filtered with Whatman No.1 filter
paper and then dried in the oven at 1100C for 8hours. The samples were crushed and passed through different sieve sizes and then stored in a tight bottle ready for use. 2.3 Characterization of activated carbon The pH of the carbon was determined using standard test of ASTM D 3838-80 . Moisture content of activated carbon and raw materials was determined using ASTM D 2867-91.The bulk density of the activated carbon was determined according to the tamping procedure by Ahmedna et al . The volatile content was determined by weighing 1.0g of sample and placing it in a partially closed crucible of known weight. It was then heated in a muffle furnace at 9000C for 10mins.The percentage fixed carbon was determined as 100 – (Moisture content + ash content + volatile matter). The iodine number was determined based on ASTM D 4607-86 ] by using the sodium thiosulphate volumetric method The specific surface area of the activated carbon was estimated using Sear’s method [13, 14] by agitating 1.5g of the activated carbon samples in 100ml of diluted hydrochloric acid at a pH = 3. Then a 30g of sodium chloride was added while stirring the suspension and then the volume was made up to 150ml with deionized water. The solution was titrated with 0.1N NaOH to raise the pH from 4 to 9 and the volume, V recorded. The surface area according to this method was calculated as S = 32V – 25. Where, S = surface area of the activated carbon, V = volume of sodium hydroxide required to raise the pH of the sample from 4 to 9. 2.4 Adsorbate preparation and batch adsorption studies The sample (Pb(NO3)2 was dried in an oven for 2hrs at 1050C to remove moisture. The simulated wastewater effluent was produced by dissolving 1.6g of Pb(NO3)2 in 1000ml of de-ionized water to get the stock solution of 1000g/l. 0.5g of activated carbon was added to 100ml of the 100mg/l of adsorbate in a conical flask and placed on a magnetic stirrer. The stirring was done at 300C for 2hrs. After adsorption was complete, the solution was filtered using Whatman no.1 filter paper. The residual Pb2+ concentrations of the effluent were determined spectrophotomically using Atomic Absorption Spectrophotometer at 217.0nm wavelength. The adsorption capacity, qe (mg/g) and percentage adsorbed were calculated from equation 1 and equation 2 respectively.
q e [(C o C e ) V / m]
% Adsorbed [(C o C e ) / C o ] x 100
1831 | P a g e
J. T. Nwabanne, P. K. Igbokwe / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 4, July-August 2012, pp.1830-1838 Where, Co and Ce are the metal concentrations (mg/l) at initial and any time t, respectively, V the volume of the solution (L), and m the mass of adsorbent used (g).
Table 1: Physico-chemical characteristics of the activated carbons
2.4.1 Effect of particle size The effect of particle size on the sorption of Pb2+ was investigated by changing the particle size in the range of 150 to 1100μm with initial concentration of 100mg/l and adsorbent dosage of 0.5g for 2hrs. 2.4.2 Effect of adsorbent dosage Initial ion concentration of 100mg/l was used in conjunction with adsorbent dosage 0.2, 0.35, 0.5, 1.0, 1.5 and 2.0g for contact time of 2hrs and particle size of 150μm.
2.4.4 Effect of contact time The effect of contact time was investigated for 10, 20, 40, 60, 90, 120, 150 and 180 min at pH 6, 0.5g/100ml sample dosage and at temperatures of 30-500C. 2.4.5 Effect of initial ion concentration The effect of initial Pb2+ concentration on the sorption was investigated by changing the initial ion concentration in the range of 100-750mg/l with 150μm particle size, adsorption dosage of 0.5g and at 30-500C for 2hrs.
3. RESULTS AND DISCUSSION Physico-chemical characteristics of activated carbons are shown in Table 1. It can be observed that OPS had the lowest moisture and ash contents and high surface area of 863m 2/g and iodine value of 810.75 mg/g. NPN had the lowest bulk density and fixed carbon, and highest surface area and iodine number. OPF had the lowest iodine number and surface area. The presence of ash has been shown to inhibit surface development . Consequently low surface area is observed in carbons with high ash content . The raw material, the particle size range used and the degree of activation affect bulk density, which does have an effect on adsorption per unit volume . The iodine number value is an indication to surface area of the activated carbon . The larger the surface area is, the greater is the adsorption capacity.
3.1.1 Effect of adsorption dosage on the adsorption process Adsorption dosage is an important parameter as it determines the capacity of an adsorbent for a given initial concentration of the adsorbate. The result showed that as the adsorbent dosage increased, the percentage of adsorption also increased but the amount adsorbed per unit mass of the adsorbent decreased considerably (Figure 1). The decrease in unit adsorption with increasing dose of adsorbent is attributed to adsorption sites remaining unsaturated during the adsorption reaction . Figure 1 reveals a definite increase in the adsorption capacity of the adsorbents with dosage. This is as a result of the larger number of available adsorption sites favouring the enhanced uptake of the metal ions . The authors stated that the dependence of adsorption on doses can be explained in terms of the concentration factor involving low metal-to-adsorbent ratio at low metal concentrations. At higher concentrations, the available sites of adsorption become fewer and hence the percentage of metal ion removed is dependent upon the initial concentration. Many workers have reported similar results [21, 22, 23]. 105
2.4.3 Effect of pH The effect of pH on the sorption was studied at pH 3, 4, 5, 6, 7, 8 with 0.5g of adsorbent dosage, for 2hrs.
3.1 Batch adsorption studies
NPN PPN EFB
Adsorbent dosage, g Figure 1: Effect of adsorbent dosage on the 2+ dosage on the adsorption of Pb Fig. : Effect of adsorbent adsorption of Pb on the adsorbents
on the adsorbents
1832 | P a g e
J. T. Nwabanne, P. K. Igbokwe / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 4, July-August 2012, pp.1830-1838 3.1.2 Effect of particle size on the adsorption process The removal of Pb2+ at different particle sizes showed that the removal rate increased as particle size deceased (Figure2). This same trend was reported by different authors [23, 24]. The relatively higher adsorption with smaller adsorbate is explained by the fact that smaller particle yields large surface area. According to Weber and Morris , the breaking of larger particles tends to open tiny cracks and channels on the particle surface of the material resulting in more accessibility to better diffusion, owing to the smaller particle size. OPS and NPN gave the best performance in removal of Pb2+ from aqueous solution. This may be attributed to their high surface areas.
Figure 3: Effect of pH on the adsorption of Pb2+ on the adsorbents 3.1.4 Effect of initial ion concentration on the adsorption process The initial metal concentration of an effluent is important since a given mass of sorbent can only adsorb a fixed amount of heavy metal. From Figure 4 it is seen that the adsorption percentage decreased with increase in initial ion concentration. However, the amount of Pb2+ adsorbed increased with increase in initial ion concentration. The lead (11) adsorbed by OPS was above 95% irrespective of the initial ion concentration as seen in Figure 4. This shows that OPS is a very good adsorbent for Pb2+ adsorption. 120
Figure 2: Effect of particle size on the adsorption of Pb2+ on the adsorbents
3.1.3 Effect of pH on the adsorption process pH is one of the most factors influencing not only site dissociation, but also the solution chemistry of heavy metal. Figure 3 presents the effect of pH on the removal of Pb2+ by the different adsorbents. The adsorption of the Pb2+ increased with increasing pH. The maximum Pb2+ adsorption for all the adsorbents was obtained at pH 6. Pb2+ adsorption decreased as pH rose beyond the optimum pH of 6. Above pH 6, Pb(II) started precipitating as Pb(OH)2. Similar result was reported by Liu et al .The increase in adsorption capacity of Pb(II) with increasing pH is attributable to two possible mechanisms, which are cation exchange and surface complexation mechanisms. At pH above 6, adsorption onto OPS was still high in comparison with other adsorbents.
60 NPN PPN EFB OPF OPS
Initial Ion Concentration, mg/l
Figure 4: Effect of initial ion concentration on the Fig. 3: Effect of initial ion concentration on the adsorption of Pb the adsorbents adsorption of Pb2+ on the adsorbents 3.1.5 Effect of contact time on the adsorption process. The result of percentage Pb2+ adsorbed is shown in Figure 5. It was found that the Pb2+ adsorption percentage increased with increasing contact time. Above 75% of Pb2+ adsorption
1833 | P a g e
J. T. Nwabanne, P. K. Igbokwe / International Journal of Engineering Research and Applications (IJERA) ISSN: 2248-9622 www.ijera.com Vol. 2, Issue 4, July-August 2012, pp.1830-1838 occurred in the first 10 to 60mins for all the adsorbents and thereafter the rate of adsorption of the adsorbate species into the adsorbent was found to be slow. The time required to reach equilibrium on Pb2+ adsorption was 90, 90, 120, 120 and 90mins for NPN, PPN, EFB, OPF and OPS respectively. The initial rapid adsorption is due to the availability of the positively charged surface of the adsorbents for adsorption of anionic Pb2+ species present in the solution. The later slow adsorption is probably due to the electrostatic hindrances between adsorbed negatively charged adsorbate species into the surface of adsorbents and the available anionic adsorbate species in solution, and the slow pore diffusion of the solute ion into the bulk of the adsorbent .
Ce 1 1 Ce qe Qob Qo
Where Ce is the equilibrium concentration of the adsorbate, q e the amount of adsorbate per unit mass of adsorbent (mg/g), and Q0 and b are Langmuir constants related to adsorption capacity and rate of adsorption, respectively. When Ce/qe is plotted against Ce, straight line with slope 1/Q0 indicates that adsorption follows the Langmuir isotherm. The Langmuir constants, Q0 and b were evaluated from the intercept and the slope of the linear plot of experimental data of 1/qe versus 1/ce and presented in Table 2 to 6. The essential characteristics of the Langmuir equation can be expressed in terms of a dimensionless separation factor, RL, defined as .
1 1 bCO
60 NPN PPN EFB OPF OPS
Contact time, min
Figure Effect of contact time the adsorption Fig. 4:5: Effect of contact time on theon adsorption of Pb onof the Pb2+ on the adsorbents adsorbents
Where, Co is the initial ion concentration, b the Langmuir’s adsorption constant (L/mg).The RL value implies the adsorption to be unfavourable (RL > 1), Linear (RL =1), favourable (O